PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses


 Della George
 11 months ago
 Views:
Transcription
1 OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft all new document correction of RF definition and added text on failure criteria
2 OPTIMAT BLADES Page 2 of 24 TABLE OF CONTENTS 1 INTRODUCTION PREDICTION PACKAGES Classical Laminated Plate package FEM package PREDICTION OF THE UD SPECIMEN PROPERTIES Materials, layup and geometry CLT results FEM results PREDICTION OF THE MD SPECIMEN PROPERTIES Materials, layup and geometry CLT results FEM results CONCLUSION AND EVALUATION REMARKS LITERATURE...24
3 OPTIMAT BLADES Page 3 of 24 1 INTRODUCTION In this note, analysis results are given for the first analyses step in WP10. This involves predictions of the specimen strain patterns and reserve factor patterns for the Optimat Blades UD and MD specimens, using literature material data. The properties have been predicted using a CLT program and a simple FEM package. The following test cases are defined in [4]: No. type loading comments direction value [N/mm] U1t UD tension longitudinal 40 U1c UD compression longitudinal 40 U2t UD tension transverse 40 U2c UD compression transverse 40 Ust UD shear tensile tbd still to be defined M1t MD tension longitudinal 40 M1c MD compression longitudinal 40 M2t MD tension transverse 40 M2c MD compression transverse 40 Mst MD shear tensile tbd still to be defined Table 1: Load cases for the specimen predictions
4 OPTIMAT BLADES Page 4 of 24 2 PREDICTION PACKAGES 2.1 Classical Laminated Plate package The Classical Laminated Plate theory has been implemented in numerous software packages. Provided the packages have been tested thoroughly, these all should give the same results. There are some differences in the completeness of the userinterface and failure criteria offered but basically the results given are the ABD matrices, strains and stresses. The package used in this report, is a demo version of 'The Laminator' [2], a relatively easy to use and cheap package. It offers possibilities of loading the (infinite) plate and calculate the strains, stresses and socalled 'Load Vector Scale Factors'. The latter gives the ratio of fracture load and applied load. In parallel calculations have been performed with the 'Kolibri' package [1] on infinite plates. This package also has a simple finite element (see 2.2) and outputs strength results as the 'Reserve Factor' (RF) or the inverse thereof. This RF seems equivalent to the 'Load Vector Scale Factors' as used by 'The Laminator'. In this document RF will be used for both packages. 2.2 FEM package The 'Kolibri' package offers the possibility of calculating the behaviour of a finite, rectangular plate when mechanically loaded. The plate can be constrained or loaded by a uniform pressure, or a point, area or edge load. For the purpose of this investigation, and edge force has been used. The package is limited in element types: only triangular elements are possible, probably with 3 nodes (no detailed information is given). The mesh can be generated automatically, or in a regular mesh. Unfortunately it is not possible to constrain the loaded edge in such a way that global translation results. Therefore halfmodels are used (half of the specimen length) in which deformation of the cross section in the specimen middle plane is allowed although this would not occur in reality. For these reasons, the package can not be seen as a highquality FEM package like Nastran or MARC. Results can be used, however, as an illustration of the stress rise near the clamped edge. In the 'Kolibri' package three failure criteria are possible: maximum strain, maximum stress and TsaiHill. In this document only the TsaiHill criterion will be reported on.
5 OPTIMAT BLADES Page 5 of 24 3 PREDICTION OF THE UD SPECIMEN PROPERTIES 3.1 Materials, layup and geometry The material properties used for the analyses are as given for the Silenka Eglass/MY750 combination, as given in [3]. No tab material is used as there are no possibilities to model a specimen including tabs and grip constraints. For some of the material properties, the complete stressstrain curve is given, since the behaviour is nonlinear. The inplane shear properties are given in Figure 1. The actual strain at failure is 4% instead of 1.25% (when using Hooke's law). This will have some consequences for the failure load predictions. For both the CLT package applied as the FEM package, nonlinar material properties are not possible. Therefore the initial moduli will be used and the failure stress as given in [3] stress [MPa] 25 full curve Hooke strain [%] Figure 1: Stressstrain curve for inplane shear For the UD specimen a simple layup is used: 4 layers of 0 oriented layers with a thickness of 0.88 mm. The geometry of the specimen is given in [3]: a straight specimen with width of 25 mm and free length of 35 mm. The nominal specimen thickness (4 layers of material) is 3.52 mm. 3.2 CLT results Specimen stiffness and FPF strength can be predicted by the CLT package. The results are easy to describe: the specimen has the stiffness and strength properties of the UD layer itself. No layers are included with different material properties or orientation, therefore the FPF strength also is the final failure strength. The failure loads are given as running loads: force by unit width.
6 OPTIMAT BLADES Page 6 of 24 E x [MPa] E y [MPa] G xy [MPa] 5830 ν xy ν yx N xt [N/mm] N xc [N/mm] 2816 N yt [N/mm] N yc [N/mm] N xy [N/mm] Table 2: CLT results for the UD specimen layup (TsaiHill criterion) 3.3 FEM results For the FEM analyses a half model has been used, see Figure 2, of the free part of the specimen outside the grips. Although the distribution of the triangular elements is not regular, this has no significant effect on the strain distributions. Figure 2: Mesh for the UD specimen, generated automatically by the Kolibri package The rectangular plate is clamped at the left side, free at the other edges and loaded by an edge loading of 40 N/mm at the right side. Due to package limitations, no constraints on the right end are applied. The FEM package has the option to rotate the laminate. This has been used to calculate the distributions when loading the laminate in the transverse direction.
7 OPTIMAT BLADES Page 7 of 24 As can be seen from the strain distributions in Figure 4, at the loaded end the specimen is not strained homogenously. This is a consequence of the short free length of the specimen. For a specimen with doubled length strains are homogeneous at the loaded end, as can be seen in Figure 3. It should be noted that the strain distributions over the first 17.5mm from the clamped side are not the same for both models. Figure 3: Longitudinal strain distribution for double length (load case U1t) The predicted patterns of the strain and the inverse of the reserve factor are given in Figure 4 to Figure 9. Peak strains always occur at the corners of the clamped side of the specimen, as can be expected. The strain values itself are also influenced by the number of elements used in the mesh. Smaller elements apparently lead to higher peak strain values. For tensile loaded cases, the inverse of the reserve factor per layer is dominated by the strain transverse to the fibre. For compression loaded cases, domination is less simple. ε x strains [%] ε y 1/RF CLT max CLT max CLT max M1t M1c M2t M2c Table 3: Strains and strength aspects of UD specimen Values for the strains and the inverse of the reserve factors, for a loading of 40 N/mm, are given in Table 3 for an infinite plate (designated 'CLT') and the extreme values for the FEM
8 OPTIMAT BLADES Page 8 of 24 models. As can be seen from the table, the peak strains in the specimen are predicted considerably higher than for an infinite pate. As a consequence, the margin to failure is much smaller.
9 OPTIMAT BLADES Page 9 of 24 Figure 4: Laminate strain distributions at load case U1t (Fx = 40 N/mm)
10 OPTIMAT BLADES Page 10 of 24 Figure 5: Reserve factor distributions for the 0 layer at load case U1t Figure 6: Reserve factor distributions for the 0 layer at load case U1c (Fx = 40 N/mm)
11 OPTIMAT BLADES Page 11 of 24 Figure 7: Laminate strain distributions at load case U2t (Fy = 40 N/mm)
12 OPTIMAT BLADES Page 12 of 24 Figure 8: Reserve factor distributions for the 0 layer at load case U2t Figure 9: Reserve factor distributions for the 0 layer at load case U2c (Fy = 40 N/mm)
13 OPTIMAT BLADES Page 13 of 24 4 PREDICTION OF THE MD SPECIMEN PROPERTIES 4.1 Materials, layup and geometry The material properties used for the analyses are as given for the Silenka Eglass/MY750 combination, as given in [3]. No tab material is used as there are no possibilities to model a specimen including tabs and grip constraints. For the MD specimen [3] a 14layer layup is used: 4 layers of 0 oriented layers with a thickness of 0.88 mm and 10 layers of 45 oriented layers with a thickness of 0.88 mm. The total layup is: (45/45/0/45/45/0/45/45/0/45/45/0/45/45). The layup is therefore not symmetrical. The geometry of the specimen is given in [3]: a straight specimen with width of 25 mm, free length of 40 mm and thickness of 6.57 mm. 4.2 CLT results The evaluated laminate is nonsymmetrical, therefore the strains in all layers with the same fibre orientation may differ. Nonzero values can be found in the Bmatrix in positions B 16 and B 26. The stiffness properties for the laminate and the laminate FPF uniaxial strengths, according to the TsaiHill failure criterion, are given in Table 4. E x [MPa] E y [MPa] G xy [MPa] 9419 ν xy ν yx N xt [N/mm] N xc [N/mm] N yt [N/mm] N yc [N/mm] N xy [N/mm] Table 4: CLT results for the MD specimen layup (TsaiHill criterion) For the load cases, as given in Table 1, different failure criteria can be compared. The results for the maximum stress, TsaiHill and TsaiWu criteria are given in Table 5. In general the differences are small for the plates in tension and shear loading. Larger differences occur for the compression loaded plates, especially for the 0 degree layer in transverse compression. In view of the large differences between the reserve factors for the 0 and 45 layer in e.g. load case 'xt', the final failure can be expected to be at a much higher load. Even more so, since the stressstrain behaviour of the 45 layer is clearly nonlinear at higher stress levels.
14 OPTIMAT BLADES Page 14 of 24 Maximum stress TsaiHill TsaiWu layer xt xc yt yc xy Table 5: Reserve factors at 40 N/mm applied load (MD specimen layup) 4.3 FEM results For the FEM analyses a half model has been used, see Figure 10. Although the distribution of the triangular elements is not regular, this has no significant effect on the strain distributions that will be shown later. Figure 10: Mesh for the MD specimen, generated automatically by the Kolibri package The rectangular plate is clamped at the left side and loaded by an edge loading of 40 N/mm at the right side. Due to package limitations, no constraints on the right end are applied. A quarter model gave slightly different results as a result of the nonsymmetrical laminate. The deformed shape for load case M1t is given in Figure 11. It clearly shows the effect of the nonsymmetrical layup
15 OPTIMAT BLADES Page 15 of 24 Figure 11: Deformed shape of the MD specimen for load case M1t The predicted patterns of the strain and the inverse of the reserve factor are given in Figure 13 to Figure 18. As can be seen in most of the transverse strain graphs (see e.g. lower graph of Figure 13) the strain at the specimen free end is not yet homogeneous. This is a result of the relative short specimen free length chosen in the project. For a specimen with twice the free length (i.e. 80 mm) the strain distribution at the middle section would be close to homogenous, see Figure 12 for load case M1t.
16 OPTIMAT BLADES Page 16 of 24 Figure 12: Transverse strain distribution for a model with double length Peak strains always occur at the corners of the clamped side of the specimen, as can be expected. The strain values itself are also influenced by the number of elements used in the mesh. Smaller elements apparently lead to higher peak strain values. As was the case for the UD specimen, for tensile loaded cases the inverse of the reserve factor per layer is clearly dominated by the strain transverse to the fibre. For compression loaded cases no simple relationship is possible between a strain component and the strength. strains [%] 1/RF ε x ε y 45 layer 0 layer CLT max CLT max CLT max CLT max M1t M1c M2t M2c Table 6: Strains and strength aspects of MD specimen Values for the strains and the inverse of the reserve factors, for a loading of 40 N/mm, are given in Table 6 for an infinite plate (designated 'CLT') and the extreme values for the FEM models. As can be seen from the table, the peak strains in the specimen are predicted considerably higher than for an infinite pate. As a consequence, the margin to failure is much smaller.
17 OPTIMAT BLADES Page 17 of 24 Figure 13: Laminate strain distributions at load case M1t (Fx = 40 N/mm)
18 OPTIMAT BLADES Page 18 of 24 Figure 14: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M1t
19 OPTIMAT BLADES Page 19 of 24 Figure 15: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M1c (Fx = 40 N/mm)
20 OPTIMAT BLADES Page 20 of 24 Figure 16: Laminate strain distributions at load case M2t (Fy = 40 N/mm)
21 OPTIMAT BLADES Page 21 of 24 Figure 17: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M2t
22 OPTIMAT BLADES Page 22 of 24 Figure 18: Reserve factor distributions for 45 layer (top) and 0 layer (bottom) at load case M2c (Fy = 40 N/mm)
23 OPTIMAT BLADES Page 23 of 24 5 CONCLUSION AND EVALUATION REMARKS Mechanical properties have been calculated for two standard Optimat Blades test specimens, on basis of assumed material properties. The stiffness and firstplyfailure strength of an infinite plate has been predicted using the Classical Laminated plate theory for linear stressstrain relationships. For the MD specimen, three failure theories have been applied: maximum stress, TsaiHill and TsaiWu. For tensile and shear loaded MD plates, the differences between the theories is small. For compression loaded plates, TsaiWu predicts higher strengths for the 45 layer and (for Xc) significantly lower strengths for the 0 layer. The FEM package used is limited in many respects, therefore the results are seen as first order approximations only. Peak stresses (or strains) are in all cases expected at the clamped end of the specimen (at the grip). The specimen length is relatively small, therefore the strains are not expected to be homogeneous in the specimen middle. Due to the high peak stresses near the grips, the predicted strength of the specimen is much smaller than the values given for the infinite plate, sometimes by a factor of 23. The MD specimen is defined as nonsymmetrical. This complicates simple modelling of the specimen. The builtup of the MD specimen has to be checked.
24 OPTIMAT BLADES Page 24 of 24 6 LITERATURE [1] Kolibri package, Kolibri Evaluation Edition, CLC TU DelftTNO, the Netherlands, see [2] 'The Laminator', version 3.1, see [3] Joosse, P.A.: "Laminae and specimen definitions for FEM analyses TG4"; TU Delft, WMCGroup, doc. OB_TG4_N002 rev2, [4] Joosse, P.A.: "Proposal for the first analysis step for WP10"; TU Delft, WMCGroup, doc. OB_TG4_N003,
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationME111 Instructor: Peter Pinsky Class #21 November 13, 2000
Toda s Topics ME Instructor: Peter Pinsk Class # November,. Consider two designs of a lug wrench for an automobile: (a) single ended, (b) double ended. The distance between points A and B is in. and the
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS
11 ELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS Biswajit Jena * * Corresponding author: biswa.tech88@gmail.com Abstract: In recent years tremendous efforts have been made in development of
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationConcentrated load introduction in CLT elements perpendicular to plane
Concentrated load introduction in CLT elements perpendicular to plane EUROMECH Colloquium 556 May 2729, 2015 Dresden, Germany Theoretical, Numerical and Experimental Analyses in Wood Mechanics http://556.euromech.org
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationIllustrating Rotating Principal Stresses in a Materials Science Course
Paper ID #706 Illustrating Rotating Principal Stresses in a Materials Science Course Prof. Somnath Chattopadhyay, Georgia Southern University Dr. Rungun Nathan, Penn State Berks Dr. Rungun Nathan is an
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationCSCE 155N Fall Homework Assignment 2: StressStrain Curve. Assigned: September 11, 2012 Due: October 02, 2012
CSCE 155N Fall 2012 Homework Assignment 2: StressStrain Curve Assigned: September 11, 2012 Due: October 02, 2012 Note: This assignment is to be completed individually  collaboration is strictly prohibited.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationPredicting Fatigue Life with ANSYS Workbench
Predicting Fatigue Life with ANSYS Workbench How To Design Products That Meet Their Intended Design Life Requirements Raymond L. Browell, P. E. Product Manager New Technologies ANSYS, Inc. Al Hancq Development
More informationDelamination in the scoring and folding of paperboard
PEERREVIEWED CONVERTING Delamination in the scoring and folding of paperboard DOEUNG D. CHOI, SERGIY A. LAVRYKOV, and BANDARU V. RAMARAO ABSTRACT: Delamination between layers occurs during the creasing
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationNonlinear Analysis Of An EPDM Hydraulic Accumulator Bladder. Richard Kennison, RaceTec
Nonlinear Analysis Of An EPDM Hydraulic Accumulator Bladder Richard Kennison, RaceTec Agenda RaceTec Overview Accumulator Experimental Testing Material Testing Numerical Analysis: 1. Linear Buckling
More informationDESIGN OF A CERAMIC HEAT EXCHANGER FOR HIGH TEMPERATURE APPLICATIONS USING SIMULATION TECHNIQUES
DESIGN OF A CERAMIC HEAT EXCHANGER FOR HIGH TEMPERATURE APPLICATIONS USING SIMULATION TECHNIUES Paulo Eduardo Batista de Mello, pmello@fei.edu.br Gustavo Henrique Bolognesi Donato, gdonato@fei.edu.br Departamento
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationLap splice length and details of column longitudinal reinforcement at plastic hinge region
Lap length and details of column longitudinal reinforcement at plastic hinge region HongGun Park 1) and ChulGoo Kim 2) 1), 2 Department of Architecture and Architectural Engineering, Seoul National University,
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationAdvanced Friction Modeling in Sheet Metal Forming
Advanced Friction Modeling in Sheet Metal Forming J.Hol 1,a, M.V. Cid Alfaro 2, T. Meinders 3, J. Huétink 3 1 Materials innovation institute (M2i), P.O. box 58, 26 GA Delft, The Netherlands 2 Tata Steel
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationChapter 2. Formulation of Finite Element Method by Variational Principle
Chapter 2 Formulation of Finite Element Method by Variational Principle The Concept of Variation of FUNCTIONALS Variation Principle: Is to keep the DIFFERENCE between a REAL situation and an APPROXIMATE
More informationAPPENDIX 1 MODEL CALCULATION OF VARIOUS CODES
163 APPENDIX 1 MODEL CALCULATION OF VARIOUS CODES A1.1 DESIGN AS PER NORTH AMERICAN SPECIFICATION OF COLD FORMED STEEL (AISI S100: 2007) 1. Based on Initiation of Yielding: Effective yield moment, M n
More informationCIVL4332 L1 Introduction to Finite Element Method
CIVL L Introduction to Finite Element Method CIVL L Introduction to Finite Element Method by Joe Gattas, Faris Albermani Introduction The FEM is a numerical technique for solving physical problems such
More informationNumerical modelling of induced tensile stresses in rock in response to impact loading
Numerical modelling of induced tensile stresses in rock in response to impact loading M.T. Mnisi, D.P. Roberts and J.S. Kuijpers Council for Scientific and Industrial Research (CSIR): Natural Resources
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationParametric analysis and torsion design charts for axially restrained RC beams
Structural Engineering and Mechanics, Vol. 55, No. 1 (2015) 127 DOI: http://dx.doi.org/10.12989/sem.2015.55.1.001 1 Parametric analysis and torsion design charts for axially restrained RC beams Luís F.A.
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationAdvances in Micromechanics Modeling of Composites. Structures for Structural Health Monitoring. Albert Moncada
Advances in Micromechanics Modeling of Composites Structures for Structural Health Monitoring by Albert Moncada A Dissertation Presented in Partial Fulfillment of the Requirements for the Degree Doctor
More information